**Geometry-related magnetic interference patterns in long SN S Josephson junctions**

**Geometry-related magnetic interference patterns in long SN S Josephson junctions**

F. Chiodi,^{1}M. Ferrier,^{1}S. Gu´eron,^{1}J. C. Cuevas,^{2}G. Montambaux,^{1}F. Fortuna,^{3}A. Kasumov,^{1}and H. Bouchiat^{1}

1*Laboratoire de Physique des Solides, UMR 8502, CNRS, Universit´e Paris-Sud, 91405 ORSAY Cedex, France*

2*Departamento de F´ısica T´eorica de la Materia Condensada, Universidad Aut´onoma de Madrid, 28049 Madrid, Spain*

3*Centre de Spectrom´etrie Nucl´eaire et de Spectrom´etrie de Masse, UMR 8609, CNRS, Universit´e Paris-Sud, 91405 ORSAY Cedex, France*
(Received 19 January 2012; revised manuscript received 20 July 2012; published 9 August 2012)

*We have measured the critical current dependence on the magnetic ﬂux of two long SN S junctions differing*
by the normal wire geometry. The samples are made by a Au wire connected to W contacts, via focused ion
beam assisted deposition. We could tune the magnetic pattern from the monotonic Gaussian-like decay of a
quasi-one-dimensional (1D) normal wire to the Fraunhofer-like pattern of a square normal wire. We explain the
monotonic limit with a semiclassical 1D model, and we ﬁt both ﬁeld dependencies with numerical simulations
of the two-dimensional Usadel equations. Furthermore, we observe both integer and fractional Shapiro steps.

*The magnetic ﬂux dependence of the integer steps reproduces as expected that of the critical current I**c*, while
*fractional steps decay slower with the ﬂux than I**c*.

DOI:10.1103/PhysRevB.86.064510 *PACS number(s): 74.45.+c, 73.23.−b, 74.40.Gh*

**I. INTRODUCTION**

A nondissipative supercurrent can be transmitted between
*two superconductors (S) through a nanometer-thin insulating*
*layer (I ), when a phase difference is imposed. Supercon-*
ducting correlations can also penetrate into a micrometer-
*long, nonsuperconducting coherent metal (N ) over lengths*
*L* *greater than ξ**S*, the superconducting coherence length in
*N. A supercurrent can then ﬂow through long (L > ξ**s**) SN S*
junctions, provided that the phase coherence is preserved in
the normal wire. The supercurrent amplitude only depends
*on the normal metal resistance, the normal metal length L,*
*and diffusion coefﬁcient D,*^{1} the latter setting the diffusion
*time through the N wire τ**D* *= L*^{2}*/D. The supercurrent thus*
reﬂects the transport mechanisms in the normal wire, and is
affected by the interference and diffraction phenomena present
in the normal metal as a result of the phase coherence. The
characteristic energy of the junction is the Thouless energy,
*also set by the same parameters: E**T h**= ¯h/τ**D* *= ¯hD/L*^{2}. The
Thouless energy not only controls the supercurrent, but also
determines the amplitude of the minigap ˜_{max}*≈ 3.1E**T h*

created in the density of states of the normal wire by the
proximity of the two superconducting contacts. In contrast to
*the superconducting gap , the minigap is fully modulated*
*by the phase difference ϕ across the normal wire, being*
*maximum at ϕ= 0 and closing completely at ϕ = π.*

We have studied the behavior of the supercurrent in long
*SN S* junctions in a magnetic ﬁeld perpendicular to the
sample plane. In a previous work,^{2} we observed that the
*maximum supercurrent, the critical current I**c*, monotonously
decreased with the magnetic ﬁeld following a quasi-Gaussian
dependence. This behavior is different from the interference
*Fraunhofer pattern usually observed, for example, in SI S junc-*
*tions, SN S junctions with L ξ**s**, magnetic SF S Josephson*
junctions, etc. This difference is induced by the different aspect
*ratios of short weak links and long SN S junctions. Indeed, in*
*SI S*junctions the thickness of the junction is limited to a few
angstroms, to permit the tunneling of Cooper pairs; similarly,
*in SF S junctions the magnetic layer thickness has to be shorter*
than a few tens of nanometers, so that Cooper pairs are not
broken by the internal exchange ﬁeld. In contrast to the wide

*and short SI S and SF S junctions, SN S junctions offer the*
interesting possibility to explore a broad range of aspect ratios,
since the length of the normal metal is only limited by the phase
coherence length, which can be as long as a few micrometers at
low temperature. In this paper we explore different geometries
*of long SN S junctions. Both monotonic and nonmonotonic*
*I**c**(B) dependencies have been observed before, but we show*
*that we can tune the I**c**(B) curve from an interference pattern*
to a quasi-Gaussian monotonic dependence by varying the
normal metal’s aspect ratio.

*Monotonic I**c**(B) dependencies have been observed in bal-*
*listic long SN S junctions, formed by a normal bidimensional*
InAs electron gas connected to superconducting Nb contacts
larger than the London screening length.^{3}Their magnetic ﬁeld
dependence resulted from the screening currents in the Nb.

On the contrary, the diffusive junctions investigated in the present work are contacted by thin disordered superconducting wires in which the magnetic ﬁeld screening is negligible. We show that the geometry-dependent magnetic ﬁeld decay can be explained taking into account only the interferences between Andreev pairs’ trajectories in the normal metal.

*As a reminder, we ﬁrst consider the case of a wide short SI S*
*junction. A magnetic ﬁeld in the SI S junction plane penetrates*
*in the insulating layer of thickness d and in the superconductors*
*nearby over a length λ**L*, the London penetration length. In a
magnetic ﬁeld *B* *= −B ˆz of vector potential A= By ˆx, the*
phase shift of the Cooper pairs tunneling at different points of
the junction width is [Fig.1(c)]

*θ(y)= 2π2e*
*h*

*d**+λ**L*

*−λ**L*

*A**x**dx* *= 2π (y)*

* *_{0} *,* (1)
*where (y) is the ﬂux through the surface S**y* *= (d + 2λ**L**) y*
*and *_{0}*= h/(2e) is the quantum ﬂux. The current is obtained*
by integrating over the junction surface the supercurrent
*density j* *= j**c**sin(δ+ θ), taking into account both the su-*
*perconducting phase difference between the contacts δ and*
the phase due to the vector potential. The critical current
*dependence on the magnetic ﬂux = B(d + 2λ**L**)w, follows*
the well-known Fraunhofer pattern, a diffraction pattern
created by the interference between the ballistic trajectories

FIG. 1. (Color online) Scanning electron microscope images of
samples WAu-Sq (a) and WAu-N (b). One can see as a clear halo the
W contamination around the superconducting contacts. (c) Scheme
*of a SI S Josephson junction. (d) Scheme of the 1D model developed.*

over the junction width:

*I**c**= I**c*(0) * *_{0}
*π *

sin
*π *

* *_{0}

*.* (2)

*If we now consider SN S junctions, we expect strong differ-*
ences between junctions containing a wide or a narrow normal
wire of similar lengths: in the wide wire the phase difference
between the trajectories comes from the phase distribution
along the junction width, while in the narrow wire, the phase
of each trajectory is mainly accumulated along the junction
length.

**II. THE SAMPLES**

*We have fabricated long SN S junctions where a Au normal*
wire links two superconducting W contacts. First, a 50-nm-
*thick Au wire is drawn by e-beam lithography and deposited*
onto a SiO_{2} *substrate. We use 99.9999% pure gold, with a*
content in magnetic impurities (Fe) smaller than 0.1 ppm.

*This ensures a long phase coherence length L** **∼ 10 μm*
below 50 mK, measured in a separated weak localization
experiment. We then deposit the superconducting contacts in
a focused ion beam (FIB). After slightly etching the Au wire
with the FIB to remove possible impurities on its surface,
we inject a metallo-organic vapor of tungsten hexacarbonyl
over the sample. This vapor is decomposed by the focused
Ga^{+} ion beam, and a disordered W alloy is deposited on
the substrate. The wires produced are composed of tungsten,
carbon, and gallium in varying proportions (in our case, the
atomic concentrations are roughly 30% W, 50% C, and 20%

Ga).^{4} The superconducting critical temperature of the wires
*produced is T**c*∼ 4 K, an order of magnitude higher than the
*bulk T**c* of W.^{5} This could be due to the inclusion of Ga,
*which is itself a superconductor with T**c*= 1 K. The critical
magnetic ﬁeld of the wires is also strikingly high: at 1 K,
*H**c*= 7 T.^{6}The W wires are 200 nm wide and 100 nm thick.

The dependence of the superconducting properties of these
wires on the deposition conditions has been investigated in
*detail in Li et al.*^{7} The superconducting gap as well as the
Abrikosov ﬂux lattice have been studied by scanning tunneling
microscopy experiments.^{8} The investigation of proximity-

FIG. 2. (Color online) Main frame: sample WAu-N normalized
*critical current vs normalized ﬂux at T* = 60 mK. Light blue line:

numerical simulation of the 2D Usadel equations, where the ﬂux has
*been rescaled by a factor of 2.5 to take into account an imperfect S/N*
interface. Inset: theoretical predictions for the aspect ratio of junction
WAu-N and perfect interfaces: the analytical result of the Usadel
*equation in the 1D limit L w (red line), the numerical simulation*
of the 2D Usadel equation (blue line), the semiclassical model for
a 1D diffusive normal wire (dotted line), and a Gaussian curve with
*σ*= 1 in the notation of Eq.(7)(dashed line). The Gaussian best
ﬁt of the experimental data, which is also a good approximation of
*the numerical Usadel result, is obtained for σ= 0.5 [as deﬁned in*
Eq.(7)]. I*c,max**= 2.4 μA.*

induced superconductivity in metallic nanowires contacted by
FIB has also been recently performed.^{9} The advantages of
this technique are the deposition of the material of practically
any shape and size, without any mask, and the good quality
of the interface created. The main disadvantage is the Ga
contamination of about 250 nm around the deposited wires.

*The SN S junctions created by FIB-assisted deposition are*
comparable to junctions created with more standard fabrication
methods. We thus recovered the general results for the voltage
vs current curves and the temperature dependence of the
critical current.^{10}

*To investigate the inﬂuence of the geometry on the I**c**( )*
dependence, we have designed two samples with different
*aspect ratios: sample WAu-Sq is 1.2 μm long and 1.75 μm*
*wide, with an aspect ratio L/w= 0.7, while sample WAu-*
*N is 1.53 μm long and 0.34 μm wide, with an aspect ratio*
*L/w= 4.5 [Figs.*1(a)and1(b)].

*The I**c**( ) normalized curves for samples WAu-N and*
WAu-Sq are shown in Figs. 2 and 3, respectively. They
illustrate the important role of the aspect ratio: sample WAu-
N displays a quasi-Gaussian decay of the critical current,
while sample WAu-Sq displays oscillations which recall a
Fraunhofer pattern.

**III. SEMICLASSICAL MODEL**

To explain the behavior of sample WAu-N, a semiclassical
model was developed.^{11}The aim is to model a long diffusive
*SN S* *junction, with w L L**φ**,L**T* (1D geometry), in a
perpendicular magnetic ﬁeld *B= −B ˆz of vector potential*

FIG. 3. (Color online) Sample WAu-Sq normalized critical cur-
*rent vs normalized ﬂux at T* = 60 mK (blue dots). A trapped ﬂux
of 4.3 G has been subtracted. Red line: numerical simulation of the
*2D Usadel equation for a junction with aspect ratio L/w= 0.7 and*
W wires inductance*L = 11.5 pH. Inset: raw data for I**c**(B), with*
*I**c,max**= 38.8 μA.*

*A**= By ˆx [Fig.*1(d)]. We suppose a sinusoidal current-phase
*relation for simplicity: j* *= j**c* *sin(δ+ θ**ij**). θ**ij* is the phase
*acquired along the trajectory starting at point i and ﬁnishing*
*at point j . δ is the phase difference between the two*
superconducting contacts, and is independent of the position
*of i and j , since in this 1D geometry one can ignore the*
dephasing along the junction width in comparison to the one
along the junction length. The total current is the average over
all possible trajectories*C**ij*:

*I* *∝ Im[e*^{i(δ+θ}^{ij}^{)} _{C}*ij**].* (3)
Considering a reference trajectory 1–2 with a phase difference
*θ**a**, we have θ**ij* *= θ**a**+ θ**ij*[see Fig.1(d)]. The critical current
*is the maximum of the current I :*

*I**c**∝ Im[e*^{i(δ+θ}^{a}^{)}*e*^{iθ}^{ij}*C**ij*]max*∝ |e*^{iθ}^{ij}*C**ij**|.* (4)
Given the great number of possible trajectories, the central
limit theorem sets the distribution of the trajectories length
*to a Gaussian distribution. The phase θ**ij*, associated with the
*trajectory ij , follows then also a Gaussian distribution. Thus*

*I**c*∼*e*^{−1/2 (θ}^{ij}^{)}^{2}^{ }^{Cij}*,* (5)
*where θ**ij* *= θ**ij* *− θ**a* *is proportional to the ﬂux **ij* in the
*surface S**ij* *deﬁned by the trajectory ij [Fig.*1(d)]:

*θ** _{ij}* =

*2e*

*¯h*

*j*

*i*

*A*_{x}*dx*−

_{2}

1

*A*_{x}*dx*

= *2e*

*¯h*

*A**x**dx= 2π *_{ij}

* *_{0}*.* (6)

Introducing Eq.(6)in Eq.(5), we ﬁnd that the critical current decays as a Gaussian function:

*I**c*∼*e*^{− ( / }^{0}^{)}^{2}^{/(2 σ}^{2}^{)}*,* (7)
*where σ*^{2}*= [S*^{2}*/S**ij*^{2} *C**ij**]/(4 π*^{2}*) and S= w × L. The Gaus-*
*sian ﬁt of sample WAu-N gives σ* *= 0.5, while in our previous*

results,^{2}*we obtained σ in the range 0.74–1.8 for aspect ratios*
*L/w*in the range 1.9–10.4.

Beyond this simple Gaussian approximation, the exact
*calculation describing diffusive trajectories from point i to*
*point j gives*^{11}

*I*_{c}*= I**c*(0)

√*π*
3

* *
* *_{0}

sinh _{π}

√3
* *
* *_{0}

*.* (8)

The small difference between this ﬂux dependence and a
Gaussian one is shown in the inset of Fig. 2. While this
model explains the origin of the quasi-Gaussian shape of
*our I**c**( ) curves, the experimental decay is faster than the*
predicted one. A more precise calculation, taking into account
the two-dimensional (2D) nature of both samples as well as
the role of imperfect interfaces, is thus necessary.

**IV. USADEL EQUATIONS**

Cuevas and Bergeret^{12}have solved the 2D Usadel equation
*for long diffusive SN S junctions with low-resistance interfaces*
and for different aspect ratios of the normal wire. A complete
*ﬁeld penetration in the normal metal (w < λ**L,N*) is assumed,
neglecting any Josephson current screening effects. Moreover
no inelastic scattering is considered. The authors found
different limits:

*(1) w L : In this 1D limit, Usadel equations can be*
solved analytically yielding a monotonous Gaussian decay of
*the ﬂux-dependent critical current: at T* *= 0, I**c**(B)/I**c*(0)∼
*e**−0.238 ( / *0)^{2}(inset of Fig.2).

*(2) w L: The analytical expression being no longer valid,*
a numerical solution of the Usadel equations needs to be found.

However, the numerical simulation still yields a monotonous
*quasi-Gaussian decay of I**c*with the ﬂux.

*(3) w L: In this case, the main effect of the ﬁeld is to*
modulate the phase over the junction width, giving rise to an
interference pattern, which is identical to a Fraunhofer pattern
*for small enough aspect ratios (L/w <0.04).*

The authors do not suppose a purely sinusoidal current-
*phase relation to start with, but calculate the complete I (δ)*
*relation of a long SN S junction. However, the wide junction*
limit corresponds exactly to the Fraunhofer pattern obtained
in the case of a sinusoidal current-phase relation.

**V. EXPERIMENTAL RESULTS**

*In agreement with the prediction of Cuevas et al. for the*
*aspect ratio L/w= 4.5, junction WAu-N does not exhibit any*
oscillating pattern (Fig.2). The ﬁeld decay cannot, however,
be ﬁtted by the numerical simulation for the corresponding
*ﬂux scale / *0: the experimental decay is faster than the
predicted one by a factor of 2.5. This can be explained by
taking into account a nonperfect interface,^{13}with an interface
*resistance R**i* *given roughly by R**i* *= 2R**N* *∼ 5
(the ratio*
*R**i**/R**N* = 2 leads to a rescaling of the perfect interface curve
by a factor of 2.3). The main effect of nonideal interfaces
is indeed to increase the dwell time in the normal metal of
the coherent pairs carrying the supercurrent, thereby leading
to a larger enclosed ﬂux. In the case of sample WAu-N, this
nonperfect interface may be attributed to the right W contact,

which is just at the extremity of the gold wire [see the scanning electron microscopy image, Fig.1(b)].

*To understand the experimental I**c**( ) of sample WAu-Sq,*
it is necessary to take into account not only the aspect ratio
of the normal wire, but also the ﬂux correction due to the
inductance of the W contacts, evident in the tilt of the central
*peak of the I**c**( ) curve. The “internal” ﬂux *intthrough the
*normal wire is thus the sum of the applied external ﬂux and*
the ﬂux created by the current ﬂowing in the superconducting
*contacts, *_{L}*= L × I**c**( *_{int}), following the relation

* *_{int}*= + L I**c**( *int*).* (9)
The experimental curve should then be compared not to
*the calculated curve I*_{c}^{th}*( *int*) but to I*_{c}^{th}*( )= I**c*^{th}*[ *int−
*L I**c*^{th}*( *_{int})]. The best ﬁt of our data for sample WAu-Sq
according to the above expression yields*L = 11.5 pH. This*
value, which we attribute to the kinetic inductance (much
*larger than the geometrical one) of the two 2-μm-long*
superconducting wires over the normal metal, is compatible
with the kinetic inductance of similarly made W wires.

When comparing our experimental results with the nu-
*merical simulation of the 2D Usadel equation for L/w= 0.7*
modiﬁed by the self-inductance, we ﬁnd good agreement in the
*position of the zeros for = BS, with S = 3.25 μm*^{2}. This
corresponds roughly to the whole surface of the normal metal
square, slightly larger than the surface between the contacts.

The amplitude of the measured oscillations following the
central peak decreases slower than predicted, and the minima
of the ﬁrst periods do not go to zero; this can be qualitatively
explained as the effect of a nonuniform current distribution in
the normal metal.^{14}

**VI. SHAPIRO STEPS**

*We have measured the differential resistance dV /dI when*
irradiating the junctions with microwaves from an antenna.

We have observed Shapiro steps, in the form of microwave-
*induced zero resistance dips at V* =_{2e}^{h}*nf*. They result from
*the resonance of the ac voltage at frequency f induced by*
the microwaves, with the current oscillations at frequency
*f*_{J}*= 2 eV/h, due to the ac Josephson effect at ﬁnite voltage*
*V* [Figs. 4(a) and 4(b)]. In addition to the Shapiro steps at
*integer n, we ﬁnd fractional Shapiro steps at n= 1/2, n = 1/3,*
*n= 3/2, and n = 1/4. In contrast to what has been observed*
by Dubos^{15} *at high temperature (T* = 4 K, corresponding
*to 13E**T h**), at T* *= 150 mK (2.4E**T h*) we still see Shapiro
*steps with n > 1 at voltages larger than the Thouless energy*
*(E**T h**/e= 5.3 μV). Moreover, we observe Shapiro steps for*
frequencies larger than the minigap ( ˜*/ h*= 4 GHz), despite
the fact that frequencies of the order of the minigap are
expected to break the pairs and create excitations above the
minigap.

*Fractional Shapiro steps appear in SN S junctions as a*
consequence of a nonsinusoidal current-phase relation. The
additional harmonics in the current-phase relation can be
generated by multiple coherent Andreev reﬂexions (MAR),
*when the coherence length is much longer than the N length, or*
by nonequilibrium effects. Fractional Shapiro steps reﬂect the
*behavior of each harmonic individually: the step at n= 1/2,*
for example, is generated by the second harmonic and is

*FIG. 4. (Color online) (a) Differential resistance dV /dI of*
*sample WAu-Sq in the presence of an irradiation at frequency f* =
*2.8 GHz. (b) dc voltage vs Shapiro step order for sample WAu-Sq;*

*the voltage was directly deduced from the measured V (I ) curves.*

*Lines show the predicted dependence V= h/2enf . (c) Normalized*
*ﬂux dependence of Shapiro steps current amplitude for n*= 1 and
*n= 1/2 (symbols) compared to the critical current dependence under*
*microwaves, which cause the reduction in I** _{c}*amplitude (continuous

*lines); the trapped ﬂux of 4.3 G, corresponding to 0.7*0, is partially

*compensated by the inductance-related tilt of the I*

_{c}*( ) central*peak.

proportional to its amplitude, having the same dependence
on ﬁeld and temperature. We have studied the magnetic ﬁeld
dependence of both integer and fractional step amplitudes. As
expected, the ﬁeld dependence of the integer Shapiro steps
follows roughly that of the zeroth-order step, the critical
current [Fig. 4(c)]. This is not the case, however, for the
fractional steps: In Fig. 4 we show that the decay with
*the normalized ﬂux of step n= 1/2 is slower than that of*
the critical current. If this fractional Shapiro step was due to
the MAR at equilibrium, the ﬁeld dependence would show
a periodicity half that of the critical current, corresponding
to the double length covered by the Andreev pairs, and the
zeros of the Fraunhofer pattern should be found at multiples of
* *_{0}*/2. This is evidently not the case, so that the supplementary*
harmonic in the current-phase relation may be traced back
to nonequilibrium effects, as already suggested in Dubos
*et al.*^{15} *and Chiodi et al.*^{16} Moreover, the effect of the
magnetic ﬁeld at the lowest temperatures was already shown to
*increase the total critical current in the out-of-equilibrium SN S*
junction.^{17}

**VII. CONCLUSIONS**

*We have measured the I**c**( ) curves for two different*
*geometries of long SN S junctions. The samples are made*
by a Au wire connected to W contacts, via FIB-assisted
deposition. We have observed a monotonic Gaussian-like

decay for a quasi-one-dimensional normal wire, in contrast
to the Fraunhofer-like interference pattern of a square normal
wire. We explain the monotonic limit with a semiclassical
1D model, and ﬁt both ﬁeld dependencies with numerical
simulations of the 2D Usadel equation. Moreover, we have
observed both integer and fractional Shapiro steps and their
dependence in magnetic ﬁeld. While integer steps follow
as expected the ﬁeld dependence of the critical current,
*fractional steps decay slower than I**c*. This is incompatible

with equilibrium MAR-originated steps, but may be explained as an out-of-equilibrium effect.

**ACKNOWLEDGMENTS**

We are grateful to M. Aprili, R. Deblock, B. Reulet, A. Chepelianskii, J. Gabelli, and I. Petkovic for fruitful discussions. This work was supported by RTRA Triangle de la Physique NanoMan and ANR QuantADN.

1T. T. Heikkil¨a, J. S¨arkk¨a, and F. K. Wilhelm,**Phys. Rev. B 66,**
184513 (2002).

2L. Angers, F. Chiodi, G. Montambaux, M. Ferrier, S. Gu´eron, and
H. Bouchiat, J. C. Cuevas,**Phys. Rev. B 77, 165408 (2008).**

3F. Rohlﬁng, G. Tkachov, F. Otto, K. Richter, D. Weiss, G. Borghs,
and C. Strunk,**Phys. Rev. B 80, 220507 (2009).**

4The concentrations are deduced with a 50% error by EDX measurement.

5W. L. Bond, A. S. Cooper, K. Andres, G. W. Hull, T. H. Geballe,
and B. T. Matthias,**Phys. Rev. Lett. 15, 260 (1965).**

6A. Yu. Kasumov, K. Tsukagoshi, M. Kawamura, T. Kobayashi,
Y. Aoyagi, K. Senba, T. Kodama, H. Nishikawa, I. Ikemoto,
K. Kikuchi, V. T. Volkov, Yu. A. Kasumov, R. Deblock, S. Gu´eron,
and H. Bouchiat,**Phys. Rev. B 72, 033414 (2005).**

7W. Li, J. C. Fenton, Y. Wang, D. W. McComb, and P. A. Warburton,
**J. Appl. Phys. 104, 093913 (2008).**

8I. Guillamon, H. Suderow, S. Vieira, A. Fern´andez-Pacheco, J. Ses´e,
R. C´ordoba, J. M. De Teresa, and M. R. Ibarra,**New J. Phys. 10,**
093005 (2008).

9J. Wang, C. Shi, M. Tian, Q. Zhang, N. Kumar, J. K. Jain, T. E.

Mallouk, and M. H. W. Chan,**Phys. Rev. Lett. 102, 247003 (2009);**

J. Wang, M. Singh, M. Tian, N. Kumar, B. Liu, C. Shi, J. K. Jain,
N. Samarth, T. E. Mallouk, and M. H. W. Chan,**Nat. Phys. 6, 389**
(2010).

10P. Dubos, H. Courtois, B. Pannetier, F. K. Wilhelm, A. D. Zaikin,
and G. Schon,**Phys. Rev. B 63, 064502 (2001).**

11G. Montambaux,arXiv:0707.0411.

12J. C. Cuevas and F. S. Bergeret,**Phys. Rev. Lett. 99, 217002 (2007).**

13J. C. Hammer, J. C. Cuevas, F. S. Bergeret, and W. Belzig,Phys.

**Rev. B 76, 064514 (2007).**

14*Antonio Barone and Gianfranco Patern´o, Physics and Applications*
*of the Josephson Effect (Wiley, New York, 1982).*

15P. Dubos, H. Courtois, O. Buisson, and B. Pannetier,Phys. Rev.

**Lett. 87, 206801 (2001).**

16F. Chiodi, M. Ferrier, K. Tikhonov, P. Virtanen, T. T. Heikkila,
M. Feigelman, S. Gu´eron, and H. Bouchiat,**Sci. Rep. 1, 3 (2011).**

17F. Chiodi, M. Aprili, and B. Reulet,**Phys. Rev. Lett. 103, 177002**
(2009).